EVALUATION OF MATERIAL STRESS-STRAIN BEHAVIOR OF
PRESSURE TUBES OF HEAVY WATER REACTORS USING FE
ANALYSIS OF RING-TENSILE TESTS
M.K. Samal1, K.S. Balakrishnan2, V. Bhasin1, K.K. Vaze1, S.Anantharaman2
1Reactor Safety Division, Bhabha Atomic Research Centre, Mumbai-400085, India
2Post Irradiation Examination Division, Bhabha Atomic Research Centre, Mumbai-400085, India
Determination of transverse mechanical properties from the ring type of specimens directly machined from the nuclear reactor pressure tubes is not straightforward because of the presence of combined membrane as well as bending stresses arising in the loaded condition. In this work, we have performed ring-tensile tests on the un-irradiated ring tensile specimens using two split semi-cylindrical mandrels as the loading device. A 3-D finite element (FE) analysis was performed in order to determine the material true stress-strain curve by comparing experimental load-displacement data with those predicted by FE analysis. We have analyzed the deformation behavior of ring-tension specimens machined from two different types of Zirconium alloy pressure tubes as used in the Indian pressurized heavy water reactors. The effect of geometry of the loading mandrel (i.e., 2-piece vs. 3-piece type of mandrel) on the load-deformation behavior of the test-setup has been studied. It was observed that the values of maximum load as well as the deformation behavior in the post-necking region differ significantly when only the geometry of the loading-mandrel is changed keeping all the other parameters same. However, finite element analysis have been able to correctly predict these variations as it takes into account of the effect of geometry, material properties as well the interaction between the mandrel and the specimen. Hence, the use of finite element method is essential in the inverse analysis procedure where the material properties can be determined from these complex test-setups.
Keywords: Ring-tension test; Finite element analysis; Zirconium alloy; Pressure tube material
Pressure tubes act as channels of heat transfer in the pressurized water type of nuclear reactors and contain the fuel bundles. These tubes are subjected to high pressure, moderate temperature and high fluence of neutrons during the reactor operation. During service, the mechanical and fracture properties of these tubes degrade due to various material ageing phenomena including those of irradiation. In order to have better mechanical and corrosion properties in the irradiated water environment and to ensure minimum absorption cross-section for neutrons, Zirconium based alloys are usually used for manufacturing of these tubes [1-2]. The manufacturing route of these pressure tubes from the ingots is also complicated with several stages of mechanical working and heat-treatment procedures. For example, the pressure tubes of current Indian pressurized heavy water reactors (PHWRs) are manufactured from quadruple-melted ingots of Zr-2.5Nb alloys . Similarly, the fuel-clad tubes are also manufactured from different types of Zirconium alloys through a series of mechanical working and heat-treatment processes. Due to the long term exposure to aggressive environments in the reactor, significant degradation in properties of the fuel-clad tubes has also been reported by various researchers in the literature [4-8].
evaluate the transverse mechanical properties from the standard tensile tests as standard specimens with sufficient dimensions cannot be machined from the pressure tubes in the circumferential direction (the radius of curvature is too small for this purpose). Similar problem is also faced by the engineers in the mechanical property evaluation of fuel-clad tubes [9-23]. Several types of geometry of specimens and the loading-mandrels were designed by various researchers world-over in order to determine the mechanical and fracture properties of these tubes satisfactorily.
A pin-loading tension (PLT) test was designed by Grigoriev et al.  to evaluate the fracture toughness of Zicaloy-2 fuel claddings. Axially notched ring specimens cut from the fuel cladding section have been tested in a way similar to that used to test compact-tension specimens. Hsu et al.  have designed an X-shaped specimen and have used it to determine the fracture toughness of the thin-walled tubular materials. In this method, two curved axially-cracked semi-cylindrical specimens (machined from the fuel-clad tubes) were glued together by epoxy adhesive to make an X-shaped specimen so as to minimize the bending effects of the loading. A modified ring tension test was carried out by Jossefson and Grigoriev  for fracture toughness testing of cladding where flattening of the ring is prevented by means of a central piece which is inserted into the ring. The central piece has almost the same dimension as that of the ring’s internal diameter. An internal conical mandrel technique has been used in Ref.  for evaluation of fracture toughness of fuel-clad tubes.
In the recent years, specimens have been machined from the fuel-clad tubes in the form of rings of small width and tested with special types of loading mandrels. In this work, a similar technique is followed for the specimens machined from the pressure tubes, which has not received much attention in literature. However, the results from these tests cannot be used directly to evaluate the material stress-strain curve. The complexities lie in (a) existence of both tensile and bending stresses in the loading cross-section due to the curvature of the specimen, (b) effect of lateral pressure and friction drag exerted by loading mandrels on the specimen, (c) geometry of the loading mandrel and the initial gap between the mandrels, (d) orientation of gauge-length of reduced cross-section of the ring-specimen with respect to the loading axis and so on.
The aim of this work is to investigate the effects of the above-mentioned factors on the load-deformation response of the ring-tension test setup with a detailed 3-D finite element (FE) analysis and develop a suitable inverse FE analysis procedure so that the mechanical properties in the transverse direction of the pressure tubes can be satisfactorily evaluated from the test data. The mechanical properties in the axial direction of the pressure tubes can also be determined from the inverse FE analysis of tensile test data obtained from testing of straight specimens machined from the axial direction of these tubes.
In this work, experiments have been conducted on the ring-type specimens machined from the pressure tubes of two different types of materials loaded with different types of mandrels and the results of load-deformation response have been compared with those of FE simulation. It can be concluded that the finite element analysis procedure of this complex loading setup should be used to evaluate the accurate transverse mechanical properties in terms of the material true stress-strain curve.
BRIEF DESCRIPTION OF THE MATERIAL, SPECIMEN AND THE RING-TENSION
In this work, specimens in the form of circular rings have been machined from both Zircaloy-2 as well as Zr-2.5%Nb pressure tubes. Both of these materials have been used in the manufacture of pressure tubes of Indian PHWRs. Zircaloy-2 have been used in older type of PHWRs whereas Zr-2.5%Nb is used now-a-days due to the important property of lower hydrogen pick-up of these alloys from the flowing coolant (i.e., heavy water) inside the pressure tubes. The chemical composition of both of these alloys is given in Table-1 and 2 respectively. It can be noted that Zr-2.5Nb alloys contains 2.58 wt. % of Nb in addition to other alloying elements. However, the wt. % of Cr and Ni are significantly lower in comparison to those of Zircaloy-2. The major alloying elements in Zr-2.5Nb pressure tubes are niobium and oxygen. Niobium is a beta stabilizer and the presence of the same in the alloys leads to the formation of a two-phase microstructure consisting of hcp α and bcc β phases. The presence of niobium in zirconium is known to increase the tensile and creep-strength of the alloy significantly. Hence, Zr-Nb alloys show improved creep resistance as compared to the other Zirconium alloys (e.g., Zircaloy-2). This is also one of the considerations for using Zr-2.5Nb alloy instead of Zircaloy-2 as the pressure tube material in the current Indian PHWRs.
Table-1: Chemical composition of Zircaloy-2 pressure tube material
Element Sn Fe Cr Ni O Zr
Wt. % 1.5 0.09 0.1 0.05 0.12 rest
Table -2 Chemical composition of Zr-2.5Nb pressure tube material
Element Al C P N O Fe Ni Cr Nb Si Sn Zr
Wt. % 0.003 0.01 0.001 0.0026 0.11 0.13 0.004 0.017 2.58 0.003 0.0056 rest
Fig. 1: (a) Ring-tension specimens with a gauge-length of reduced cross-section machined from Indian PHWR pressure tubes and tested to failure in the ring-tension setup; (b) Solid model of the ring-tension specimen, the symmetric form of which was used in FE analysis
directions are of the order of 0.58, 0.39 and 0.03 respectively . Hence, the mechanical properties of these tubes are highly anisotropic.
The tensile specimens have been machined from the as-manufactured tubes and tested in a ring-tension setup. The pictures of the tested specimen are shown in Fig. 1(a). The 3-D solid model of the specimen used in the FE analysis is shown in Fig. 1(b). The rings machined from the Zircaloy-2 pressure tube have internal diameter values of 83 mm and the value of thickness as 4.3 mm, whereas for the rings machined from Zr-2.5Nb pressure tubes, the corresponding dimensions are 83 mm and 3.6 mm respectively. A section of the ring specimen has a reduced cross-section (known as gauge-length section) in order to induce necking in the same region. The width of both of the ring specimens is 6 mm in the gauge-length section and 12.5 mm away from the gauge-length section. The specimen having a single reduced gauge-length in the periphery is also known as the single-gauge-length (SGL) specimen. The gauge length has a dimension of 25 mm in case of the Zircaloy-2 ring-specimen, whereas it is of 20 mm in case of the Zr-2.5Nb ring-specimen. The gague-length can be oriented at different angles with respect to the loading axis of the testing machine. When the gauge-length is oriented at right angle to the loading axis, the arrangement is known as “12 ‘O’ clock position” in this paper.
The ring-tension setup consists of the ring-specimen and the loading mandrel. The loading mandrel can be of various designs. We have considered two types of loading mandrels (i.e., 2-piece and 3-piece type of mandrel) in this work. The 2-piece mandrel consists of two semi-cylindrical mandrels with a gap between them and they load against the ring-specimen with the help of loading pins. In case of the 3-piece mandrel, a central piece is inserted in between the top and the bottom loading mandrels in order to restraint the lateral movement of the ring-specimen during loading. The loading arrangements with the 2-piece and 3-piece mandrels are shown in Fig. 2(a-c) respectively.
(a) (b) (c)
Fig. 2: Ring specimen with gage-length oriented at 12’O clock position in the test grips. (a) 2-piece mandrel, pins and the loading grip before assembling the parts; (b) 2-piece mandrels fitted with ring specimen loaded in the grips; (3) 3-piece mandrels fitted with ring specimen loaded in the grips
FINITE ELEMENT ANALYSIS OF RING-TENSION SETUP
20-noded iso-parametric brick elements with tri-quadratic interpolation functions for the nodal variables (i.e., displacements in three Cartesian co-ordinate directions). The von Mises yield condition along with the Prandtl-Reuss flow rule have been used as the constitutive model for the elastic-plastic FE analysis.
Fig. 3: FE mesh of the ring-tension setup. SGL specimen with (a) 2-piece loading mandrel, (b) 3-piece loading mandrel. 3-D elements for both specimen and mandrel with contact elements at the interface have been used in the analysis
0.00 0.05 0.10 0.15 0.20 0.25
400 500 600 700 800 900
Zircaloy-2 Zr-2.5% Nb
true plastic strain
Fig. 4: True stress-strain curves of pressure tube material of Indian PHWR (Zircaloy-2 and Zr2.5%Nb)
0 1 2 3
0 5000 10000 15000 20000 25000 30000
displacement (mm) 2-piece mandrel, 12 'O' clock pos.
exp. FE analysis
0 1 2 3
0 5000 10000 15000 20000 25000 30000
displacement (mm) 3-piece mandrel, 12 'O' clock pos.
exp. FE analysis
Fig. 5: Load-displacement response of the Zircaloy-2 ring-tension specimen with Zircaloy-2-piece loading mandrel and gauge-length oriented perpendicular to loading axis (exp vs. FE analysis)
Fig. 6: Load-displacement response of the Zircaloy-2 ring-tension specimen with 3-piece loading mandrel and gauge-length oriented perpendicular to loading axis (exp vs. FE analysis)
RESULTS AND DISCUSSION
The objective of this work has been to study the effect of geometrical design of the loading mandrels and the contact condition between the mandrels and the ring-specimen on the load-deformation behavior of the test setup. For this purpose, two types of loading mandrels have been considered in the experiment and their subsequent FE analysis. Two types of Zirconium alloys having significantly different mechanical properties have been considered in this work. The purpose is to test the validity of this approach for materials with widely varying stress-strain behavior. The material true stress-strain curve (in terms of true stress vs. true plastic strain) is required for FE analysis of the test setup. As the ring-tension tests are done at room temperature, the above data is required for the materials at room temperature and the same are shown in Fig. 4 for Zircaloy-2 and Zr-2.5%Nb respectively.
The yield stress (YS) and ultimate tensile strength (UTS) values of Zircaloy-2 are given as 554 MPa and 605.8 MPa respectively. The values of the above parameters are 720 MPa and 842 MPa respectively for the material Zr-2.5%Nb. It may be noted from Fig. 4 that Zr-2.5%Nb exhibits significant plastic strain hardening before the strength level reaches UTS compared to Zircaloy-2. However, plastic strain value at UTS for Zr-2.5%Nb is significantly lower (i.e., 0.028) compared to that of Zircaloy-2 (i.e., 0.047) which indicates that Zr-2.5%Nb has a lower uniform ductility compared to that of Zircaloy-2. In the post-necking region of deformation, the plastic strain hardening behavior of Zr-2.5%Nb is lower compared to that of Zircaloy-2 as can be seen from the slopes of the material stress-strain curves (beyond the UTS region) in Fig. 4. The material stress-strain curves as depicted in Fig. 4 have been used in the FE analysis as an input. The load-displacement curve of test setup can be determined from FE analysis using the procedure as discussed below.
original load-displacement data as obtained from the testing of SGL ring-specimens have been corrected by taking into account of the machine compliance as determined from the above procedure. The load-displacement response of the test-setup with 2-piece loading mandrel and the Zircaloy-2 ring (with the gauge length oriented at 12 ‘O’ clock position) as obtained from FE analysis has been plotted in Fig. 5 along with the experimental load-displacement data.
It may be noted that FE analysis has been able to correctly predict the experimental yield load, maximum load as well as the post-necking behavior very accurately. The load-deformation behavior in a problem with contact type of boundary conditions can be quite complex due to making and breaking of contact at the interfaces of the loading mandrel and the ring-specimen. As the outside curvature of the loading mandrel (with the Teflon tape on it) is nearly same as that of the inside curvature of the ring specimen, there is a surface-to-surface contact of nearly 180 degree angle (in case of 2-piece type of loading mandrel) at the beginning of loading. The gauge-length portion of the ring specimen rests on the mandrel and is subjected to extension in the circumferential direction due to relative movement of the two mandrels. The extension in the gauge-length section of ring specimen develops due to the indirect loading conditions because of the contact constraint of the mandrels exhibited with respect to the ring specimen. Once the gauge-length section starts to deform uniformly, there will be alteration in the contact conditions. However, significant effect of the change in contact conditions between the mandrel and the gauge-length section can be observed once necking sets in.
The necking of the gauge-length results in significant reduction in cross-section and the interface contact condition breaks and the necked-region now starts deforming independently. However, the contact condition still prevails in the other regions of ring-specimen away from the necked-region in both sides of the loading axis. Till necking, the mandrel exerts a lateral pressure as well as a friction drag on the lower contact surface of the ring cross-section (in the gauge-length region) and this will have significant effect on yield behavior of the specimen. It may be noted that the direction of lateral pressure is normal to the contact surface and hence, it is parallel to the loading direction, whereas the friction drag has two different directions on both sides of the loading axis as the direction of relative motion between the loading mandrel and the ring-specimen changes. The specimen gauge-length tries to move to the left hand side relative to the mandrel in the left hand side of the loading axis, whereas the motion is exactly opposite in the right hand side of the loading axis.
As the values of friction drag as well as lateral pressure depend nonlinearly on the displacement of the loading mandrel, these are very difficult to estimate in a closed form solution of the elastic-plastic deformation behavior of the test setup. However, the FE analysis used in this work has been very well able to simulate the accurate contact conditions and hence, the resulting load-displacement curve for the whole displacement range compare very well with that of experiment as shown in Fig. 5. The FE analysis has then been carried out for the test-setup with 3-piece loading mandrel. The gauge-length of the SGL ring-specimen is also aligned in 12 ‘O’ clock position in this experiment. The load-displacement result of FE analysis of the test-setup with 3-piece mandrel has also been compared with that of experiment in Fig. 6 and the FE result is very close to that of experiment in the whole range of deformation.
because the effect of friction and contact boundary conditions existing at the interface of the specimen and the loading mandrel are not taken into account in the calculation of engineering stress and engineering strain in the standard equations. It is also not possible to introduce the above effects in a closed form equation because of the complexities involved as discussed earlier. Hence, a 3D FE analysis with capability to handle the above effects is essential for accurate estimation of material stress-strain curve through an inverse analysis procedure.
0 1 2 3
0 5000 10000 15000 20000 25000 30000 35000
3-piece mandrel, 12 'O' clock pos. exp.
Fig. 7: von Mises equivalent plastic strain contour in the Zr2.5%Nb ring-tensile specimen loaded with 3-piece mandrel for an applied displacement of 3 mm
Fig. 8: Load-displacement response of the Zr2.5%Nb ring-tension specimen with 3-piece loading mandrel and gauge-length oriented perpendicular to loading axis (exp vs. FE analysis)
It may be noted that the FE analysis is able to successfully predict the different values of maximum load as well as the post-necking behavior of the two test-setups with a single data of material stress-strain curve as the input. Hence, the inverse FE analysis is able to estimate the same material stress-strain curve from the two different types of tests albeit prediction of completely different load-displacement responses and hence, it acts as a true transfer function between the material response (dependent only upon material property and independent of geometry of specimen and loading mandrel) and the system response. The calculation procedure of engineering stress and strain is also not straight forward as the deformation in a ring is similar to deformation in a statically indeterminate system. This is because of redistribution of load and deformation along the circumference of the ring during loading as the ring is continuous. For this purpose, the engineering stress at the gauge section of the ring is calculated by dividing the half of the total load (as the load is shared equally between the two diametrically-opposite cross-sections of the ring, though these are of different values of cross-sectional area) by the area of cross-section of the gauge section (i.e., with reduced value). Similarly, the engineering strain is calculated by dividing the twice of the displacement magnitude of the loading mandrel (the two vertical legs of the ring being deformed simultaneously due to the relative movement of the mandrels) with the gauge length of the ring-specimen.
von Mises equivalent plastic strain is 73.5% approximately (Fig. 7). However, the engineering strain as calculated from the applied displacement (2x3 mm) and the gauge length (20 mm) is around 30%. This is because of the presence of multi-axial deformation and hence, a multi-axial state of stress in the necked-region. The calculation of engineering strain (as 30%) is valid for a pure uni-axial deformation case.
Fig. 7 also shows that the contact between the middle loading mandrel and the specimen breaks on both sides of loading axis and hence, the contact conditions are significantly different in comparison to that of a 2-piece mandrel where the contact remain intact in approximately 180 degree angle of the loading mandrel throughout the deformation history (except the portion of necked-region after necking has started). The load-displacement response of the test-setup with 3-piece mandrel and the Zr2.5%Nb ring-specimen as been determined from FE analysis has been compared with that of experiment in Fig. 8. It may be noted that the FE analysis has also been able to satisfactorily predict the experimental load-displacement behavior of this test-setup for a different alloy. Hence, the procedure is validated and this gives confidence in the use of this combined FE analysis and experimental procedure for accurate estimation of transverse mechanical properties of the Zircaloy pressure tubes in the as-manufactured as well as in the service-exposed conditions, which is very crucial for the design as well as safety analysis of these components.
Use of ring-specimens for evaluation of mechanical properties in the as-received as well as service-exposed conditions of nuclear reactor pressure tubes is very attractive due to the ease of machining of the specimens and testing in different conditions including those of irradiation. However, the mechanical properties cannot be directly evaluated due to complexity of the test-setup. In this work, a 3-D FE analysis procedure has been adopted and it was shown that it is possible to estimate the load-displacement response of the test-setups accurately by taking into account of the variability in mandrel design and contact conditions. The dynamic nature of evolution of contact conditions during loading and hence, the effect of additional stresses (i.e., those due to lateral pressure and interface drag) on the yield and subsequent material strain-hardening behavior cannot be taken care of in standard empirical equations as used for uni-axial tensile tests. Hence, use of a 3-D FE analysis (as used in this work) is recommended for accurate estimation of material properties from these ring-tension tests. The scope of future work includes assessment of the above procedure for other engineering materials such as low-alloy steels and for other tubular components used in different engineering applications.
1. Nikulina, A.V. Zirconium-Niobium Alloys for Core Elements of Pressurized Water Reactors. Metal
Science and Heat Treatment 2003; 45(7-8): 287-292.
2. Nikulina, AV. Zirconium alloys in nuclear power engineering. Metal Science and Heat Treatment
2004; 46(11-12): 458-462.
3. V. Deshmukh, U. Singha, S. Tonpe, N. Saibaba. Effect of process variables on texture and creep of pressurized heavy water reactor pressure tubes. Transactions of the Indian Institute of Metals 2010; 63(2-3): 397-402.
4. Edsinger, K., Davies, J.H., and Adamson, R.B. Degraded fuel cladding fractography and fracture
behaviour. Ziconium in nuclear industry: 12th International symposium, ASTM STP 1354. G.P. Sabol and G.D. Moan, Eds., Americal Society for Testing and Materials, West Conshohocken, PA, 2000, 316-339.
5. Murty K. L. Deformation, texture and microstructure- property correlation and in-reactor
6. Murty, K. L. Texture based physical, mechanical and corrosion characteristics of Zirconium alloys. Textures in Materials Research, Oxford and IBH co. Ltd, New Delhi, 1999, 113-126.
7. Wang, Y. and Murty, K. L. Effect of temperature on mechanical anisotropy of re-crystallized
Zircaloy-4 sheet. Proc. 4th Asia-Pacific symposium on Advances in Engineering plasticity and its applications, AEPA 98, Seoul, South Korea, 21-25 June 1998.
8. Leclercq S., Parrot A., and Leroy M. Failure characteristics of cladding tubes under RIA conditions. Nuclear Engineering and Design 2008; 238(9): 2206–2218.
9. Arsene, S., and Bai, J. A New Approach to measuring transverse properties of structural tubing by a ring test. J. Testing Evaluation 1996; 24(6): 386-391.
10. Bae, B.-K., Cho, S.-K., Seok, C.-S. A study on ring tensile specimens. Materials Science and
Engineering 2008; A483-484: 248-250.
11. Seok, C.S., Bae, B.K., Koo, J.M., Murty, K.L. The properties of the ring and burst creep of ZIRLO cladding. Engineering Failure Analysis 2006; 13: 389-97.
12. Lee,K.W., Hong, S.I. Zirconium hydrides and their effect on the circumferential mechanical
properties of Zr-Sn-Fe-Nb tubes. Journal of Alloys and Compounds 2002; 346: 302-307.
13. Bertolino, G., Meyer, G., and Perez, I.J. In-situ crack growth observation and fracture toughness measurement of hydrogen charged zircaloy-4. J. Nucl. Mater. 2003; 322: 57-65.
14. Fukuda, T., Itagaki, N., Kamimura, J., Mozumi, Y. and Furuya, T. Fracture toughness of hydrogen-absorbed zircaloy-2 cladding tube. European Nuclear Society, Topfuel 2003, Wurzburg, Germany, 16-19 March 2003.
15. Videm, K. and Lunde, L. Stress corrosion cracking and growth formation of pellet-clad interaction defects. Ziconium in nuclear industry: 4th International symposium, ASTM STP 681. J.H. Schemel and T.P. Papazoglou, Eds, Americal Society for Testing and Materials, West Conshohocken, PA, 1979, 230-237.
16. Lee, K.W., Kim, S.K., Kim, K.T., Hong, S.I. Ductility and strain rate sensitivity of Zircaloy-4 nuclear fuel claddings. Journal of Nuclear Materials 2001; 295: 21-26.
17. Grigoriev, V., Josefsson, B. Rosborg, B. and Bai, J. A novel fracture toughness testing method for irradiated tubing-experimental results and 3D numerical evaluation. Transactions of the 14th Int. Conference on Structural Mechanics in Reactor Technology, Lyon, France, 1997, 57-64.
18. Nakatsuka, M., Kubo, T. and Hayashi, Y. Fatigue Behavior of Neutron Irradiated Zircaloy-2 Fuel
Cladding Tubes. Ziconium in the Nuclear Industry: Ninth International Symposium, ASTM STP 1132, C.M. Eucken and A.M. Garde Eds., American Society for Testing and Materials, 1991, 230-245.
19. Yoshitake T., Abe Y., Akasaka N., Ohtsuka S., Ukai S. and Kimura A. Ring-tensile properties of
irradiated oxide dispersion strengthened ferritic/martensitic steel claddings. Journal of Nuclear Materials 2004; 329-333: 342–346.
20. Grigoriev, V., Josefsson, B., Lind, A. and Rosborg, B. A pin-loading tension test for evaluation of thin-walled tubular materials. Scripta Metallurgica et Materialia 1995; 33(1): 109-114.
21. Hsu, H.H., Chien, K.F., Chu, H.C., and Liaw P.K. An X-specimen test for determination of thin
walled tube fracture toughness. Fatigue and Fracture Mechanics: 32nd Volume, ASTM STP 1406, R. Chona, Ed.. Americal Society for Testing and Materials, West Conshohocken, PA, 2001, 214-226.
22. Josefsson, B., and Grigoriev, V. Modified Ring Tensile Testing and a New Method for Fracture
Toughness Testing of Irradiated Cladding. Studsvik Material AB, S-61182, Nykoping, Sweden, May 22, 1996.
23. Sainte Catherine, C., Le Boulch, D., Carassou, S., Ramasubramanian, N. And Lemaignan, C. An